However, as the experiment consisted of subsequent lithium deposition and analyzing steps, the reaction between the electrolyte and lithium does not necessarily have to be finished during the analyzing step and might still proceed during the measurement if enough lithium is present. To clarify whether the decomposition is an ongoing process, one would have to perform several measurements with different analyzing times between each lithium deposition step and see whether the intensity ratio changes over time.
Figure 30: Attenuation of total P signal. Once the SEI has reached a stable thickness, the slope of the curve can be used to calculate the deposition rate of the Li/Li2O overlayer.
The average effective attenuation length of the overlayer can be calculated from its stoichiometry (Table 8). In equation 35, m is the slope of the photoemission intensities for all P species. The thereby determined value rmix is the deposition rate of the Li/Li2O mixture, which now needs to be corrected for the Li2O component. For long deposition times, this mixture has a constant composition of XLi2O = 20 – 25 mol% as determined from the ratio of the intensities of the O 1s signal of Li2O and the total Li signal. This ratio was calculated as an average value from data recorded from 3000 s of Li deposition time until the end of the measurement, assuming that at this point mainly the overlayer contributes to the signal.
Consequently, the damping of the P 2p intensity is also caused by both Li and Li2O. It has to be noted that the EALs of O 1s and Li 1s are different. Therefore, the damping of the intensity caused by these components is different. In the case of “LiPO” and LiPON–low where a thick overlayer is assumed, these difference lead to negligible errors of the SEI composition and growth. In the case of LiPON–high, where the reaction proceeds longer than for the other two samples, the overlayer is thinner and therefore the different EALS in
the overlayer may cause a bigger error. However, this error may be smaller than the error of the SEI stoichiometry derived from the data fitting.
Table 8: Mol percentage of Li2O in the lithium overlayer calculated from the Li2O(O 1s) and (Li 1s) signals after 3000 s of Li deposition time till the end of the measurement; and average EAL thereof.
Material mol% Li2O EALP 2p ∙ cos 45° / nm
“LiPO” 17.9 3.33
LiPON–low 17.2 3.34
LiPON–high 21.9 3.27
From rmix and XLi2O, the growth rate of pure Li metal can be calculated. The volume fractions of the overlayer components can be calculated from the molar fractions with XLi2O, = ILi2O(O 1s)
ILi(total) , the ratio of the intensities of the O 1s signal of Li2O and the total Li signal.
The approximation via the oxygen signal is necessary because the intensity of the Li signal is too small to be fitted with multiple signals and to determine the fraction of Li(Li2O).
The damping of the P 2p intensity is caused by both Li and Li2O and the growth rate in equation 35 is the growth rate of the Li2O/Li layer. From this value, the growth rate of pure Li metal can be calculated. The volume fractions of the overlayer components can be calculated from the atomic fractions using the molar volumes VM,i:
VLi2O = XLi2O ∙ VM,Li
Vtotal = VLi2O+ VM,Li∙ (1–XLi2O) = VLi2O + VLi (37) A certain amount of the growth rate rmix is caused by Li2O
rmix = rLi + rLi2O, (38)
rLi2O = VLi2O
Vtotal ∙ rmix (39)
Combining (34),(37) and (38) leads to rLi = rmix – rLi2O= rmix –VLi2O
Vtotal ∙ rmix = m ∙ LOverlayer ∙ (1–VLi2O
Vtotal) ∙ 60s/min = rLi,late (40) Adding the factor 60s/min results in a more convenient growth rate per minute. As discussed above, the thermodynamic driving force for the reaction between lithium and the electrolyte
is bigger than for the reaction of lithium and oxygen or water. The formation of Li3PO4 (and Li3N) out of “LiPO(N)” is thermodynamically more favorable than the formation of Li2O from the elements (Table 7). If the formation of Li2O and/or LiOH is due to the reaction of lithium with water in the deposition chamber, the resulting reaction enthalpy is –303.0 kJ and the reaction with the chamber atmosphere instead of the electrolyte should be even less favorable. Therefore, it can be concluded that the reaction rate for forming Li2O from residual oxygen in the chamber atmosphere will be negligible as long as impinging lithium can instantaneously react with the electrolyte surface. As a consequence, lithium that would form Li2O for higher deposition times will react with the electrolyte at the beginning of the experiment. Therefore, the deposition rate of active lithium will be higher for the first deposition steps and the rate needs to be corrected. As the overlayer consists of x mol% Li2O and (100 – x) mol% Li, and for each Li2O molecule two lithium atoms are needed, the total fraction of Li is therefore (100 – x + 2 x) % = (100 + x) % of the value determined via XPS, leading to a correction factor of 100 + x
100 – x for the lithium deposition rate at the beginning of the experiment.
rinitial = rlate ∙ 100 + x 100– x (41)
In the intermediate region where the kinetic limitation of the SEI formation starts to decrease the deposition rate of active lithium, an average deposition rate will be between the values from equation 40 and equation 41. A precise value cannot be calculated, leading to a slightly erroneous value of the total lithium thickness.
For a precise determination of the thickness of the lithium layer, it is important to determine the time after which a transition from the initial to the late deposition rate sets in. A helpful indicator for this transition point is the ratio of total intensities of the oxygen and phosphorous signals in the course of the in situ experiment (Figure 31). Without additional oxygen from the residual atmosphere, this ratio should be constant in SE and SEI. Additional oxygen, however, will form Li2O on top of the sample whereas all phosphorous species stem from SE and SEI and their signal intensities are attenuated once the top–layer begins to form.
Consequently, the O/P intensity ratio reacts extremely sensitive to the formation of additional Li2O as can be seen in Figure 31.
In this figure, it can be seen that the ratio is almost constant during the first 600 s of lithium deposition time before increasing to a ratio of almost 10. In the beginning all lithium directly reacts with „LiPON“ and no oxygen from the atmosphere is trapped. Minor changes of the ratio are attributed to parts of lithium oxide that originate from the oxidized surface of the lithium foil that was used for lithium deposition. The following increase of the O/P ratio is due to the subsequent formation of additional Li2O (whose intensity is proportional to (1 — e—d)) due to kinetic limitations caused by the growing SEI and the exponential decay of the P intensity that is buried under Li2O. To summarize, the increase of the O/P ratio sets in at the time when the interphase growth of the sample LiPON–high changes from a reaction–controlled mechanism to a diffusion–controlled mechanism as will be discussed below in further detail.
After SEI formation, the Li metal film is partly oxidized by oxygen or water traces and for all samples an average composition and an average electron attenuation length could be determined. The values are summarized in Table 9.
Figure 31: Evolution of the O/P intensity ratio of the LiPON–high sample depending on the lithium deposition time. The ratio starts to increase when the reaction–
controlled interphase formation turns into a diffusion–controlled process and lithium has enough time to trap water from the chamber atmosphere. Note that this ratio does not describe the elemental composition as O and P signals stem from different depths leading to much higher intensities from surface–near species (Li2O) compared to signals from the SE and SEI.
0 2000 4000 6000
0 1 2 3 4
dSEI / nm
Lithium deposition time / s
2 4 6 8
For the calculation of the average effective electron attenuation lengths of the SEI, the average SEI composition is required. The average SEI composition determined from XPS measurements will always be erroneous, as the information depth during each measurement step is bigger than the SEI thickness created during the previous Li deposition step. At short deposition times and very low SEI intensities, the ratio is adulterated by the high intensity of the electrolyte signals. After long deposition times, the incorporation of additional Li2O falsifies the results. For that reason, the average EALs were calculated from the ratio of SEI signals at Li deposition times of 540 s – 1080 s. As the ratio of LiP is always < 3 %, it is neglected in these calculations.
Table 9: SEI composition, electron attenuation lengths of different SEI species and average values of the interphases calculated from the data after 540 s – 1080 s of lithium deposition time.
The EAL is always dependent on the emission angle 𝜃 and therefore subject of the respective XPS machine. The values given in Table 9 are corrected by the emission angle of the machine used in this work. The EAL for the three different SEIs are quite similar. The differences of the stoichiometry are small as oxygen is only replaced by nitrogen when the stoichiometry is changed. The main difference is caused by the variable amount of Li3PO4 that is formed and the average EAL is always in between the values of Li2O and Li3PO4. To evaluate the plausibility of these estimations, it is necessary to compare the obtained values to the
Species 𝐎𝐋𝐢𝟐𝐎 𝐏𝐋𝐢𝟑𝐏𝐎𝟒 𝐏𝐋𝐢𝟑𝐏 𝐍𝐋𝐢𝟑𝐍 LiLi
EALP 2p ∙ cos 45° / nm 2.29 2.41 2.29 2.28 3.59
Vol%LiPO 32.4 51.2 16.4 0 0
Vol%LiPON–low 37.0 43.0 9.9 9.2 0
Vol%LiPON–high 18.3 51.5 10.5 19.6 0
EAL SEILiPO 2.35
EAL SEILiPON–low 2.34
EAL SEILiPON–high 2.35
theoretical maximum SEI thickness obtained after the deposition of a certain amount of lithium.